Framing of Poly(arylene-ethynylene) around Carbon Nanotubes and Iodine Doping for the Electrochemical Detection of Dopamine

Dopamine (DA), an organic biomolecule that acts as both a hormone and a neurotransmitter, is essential in regulating emotions and metabolism in living organisms. The accurate determination of DA is important because it indicates early signs of serious neurological disorders. Covalent organic frameworks (COFs) and metal–organic frameworks (MOFs) have received considerable attention in recent years as promising porous materials with an unrivaled degree of tunability for electrochemical biosensing applications. This study adopted a solvothermal strategy for the synthesis of a conjugated microporous poly(arylene ethynylene)-4 (CMP-4) network using the Sonagashira–Hagihara cross-coupling reaction. To increase the crystallinity and electrical conductivity of the material, CMP-4 was enveloped around carbon nanotubes (CNTs), followed by iodine doping. When used as an electrochemical probe, the as-synthesized material (I2-CMP-CNT-4) exhibited excellent selectivity and sensitivity to dopamine in the phosphate-buffered solution. The detection limits of the electrochemical sensor were 1 and 1.7 μM based on cyclic voltammetry (CV) and differential pulse voltammetry (DPV).


Introduction
Dopamine (DA) is a neurotransmitter consisting of a catechol moiety (a benzene ring with two hydroxyl groups at the ortho-position), with one amine group attached via an ethyl chain. In 1958, Carlsson et al. discovered the neurological messenger function of DA, which generates impulses between neurons [1,2]. As a significant element in the human nervous system, DA is necessary for maintaining the neurological health of an individual. Thus, the accurate and selective sensing of DA is essential for physiological purposes. There are several enzyme-antibody aptamer-based fluorescent biosensors and electrochemical methods such as cyclic voltammetry (CV), differential pulse voltammetry (DPV), and aptamer-based colorimetric biosensors are popular for detecting DA because of their quick response and high selectivity [3][4][5][6][7][8][9][10]. The electrochemical detection of DA is favored at pH 7 because it becomes positively charged and can be easily oxidized [11,12]. Recently, multiphoton microscopy has been used to image DA with excitation at 550 nm [13][14][15]. However, uric acid (UA) and ascorbic acid (AA) usually interfere with the fluorescence and electrochemical detection of DA, owing to their structural similarities. Therefore, specific ligands and tuned frameworks are required to selectively distinguish and sense DA from its interferents and analogs.
In this scenario, electrochemical biosensors have been broadly investigated for the sensing and monitoring of neurotransmitters, owing to their high selectivity as well as the possibility of achieving real-time measurements [16]. For this purpose, electrodes made of noble metals (typically platinum or gold), carbon materials, metal oxides, metal-organic Scheme 1. Hopping and tunneling mode of charge transfer mechanism in SSOPMs. Based on the preceding characteristics, we synthesized a COF-CNT composite of a conjugated microporous poly(arylene-ethynylene)-4 network (CMP-CNT-4) through the Sonagashira-Hagihara cross-coupling reaction [27]. The enveloping of CMP-4 around the CNT provides a tubular organic crystalline framework that can enhance unidirectional charge delocalization (Scheme 2). The doping of I 2 into CMP-CNT-4 boosted the electrochemical sensitivity of the entire composite towards DA through the hopping charge transfer mechanism (Scheme 3). The morphological, optical, and chemical properties of the I 2 -CMP-CNT-4 nanocomposite were investigated using various characterization techniques, such as X-ray diffraction (XRD), scanning electron microscopy (SEM), transmission electron microscopy (TEM), Fourier transform infrared (FT-IR) spectroscopy, ultraviolet-visible (UV-Vis) absorption spectroscopy, Raman spectroscopy, X-ray photoelectron spectroscopy (XPS), and nuclear magnetic resonance (NMR) spectroscopy. Voltammetry investigations were performed using a WizMac WizEIS-1200 Premium voltammeter.

Experimental Section
Herein, we utilized a solvothermal method for the synthesis of brown-colored CMP-4 and CMP-CNT-4 networks by reacting 1,4-diethynylbenzene and 1,3,5-tribromobenzenebased linkers in toluene as the solvent ( Figure S1, ESI †). The wrapping of CMP-4 around the CNT was conducted using a minor modification of a previously reported method by dispersing CNTs into the reaction mixture, as shown in the electronic Supplementary Information. In addition, the gravimetric iodine adsorption method was used to dope I 2 vapors on the CMP-CNT-4 surface.
All chemicals and solvents were purchased from commercial suppliers and used without further purification. Solid-state 13C and 1H NMR spectra were recorded on a Bruker Advance III HD (Bruker, Germany) 500 MHz spectrometer; chemical shifts are represented in δ (ppm units). Powder X-ray diffraction (PXRD) patterns of the samples were measured using a Smart Lab instrument (Rigaku) with D/teX Ultra 250 detectors under a 4-kW X-ray generator (scan range: θ/2θ = 5-80 • ). Fourier transform infrared spectra were recorded in the range of 200-4000 cm −1 on Vertex 70 (Bruker, Billerica, MA, USA). Powder samples were dried, and subsequently, a small amount of the powder was placed directly between two support plates without hygroscopic materials (such as NaCl or KBr). SEM images were acquired from a Hitachi S-4700 FE-SEM (Japan). For all samples, imaging was performed in a high vacuum at an accelerating voltage of 15 kV, working distance of 11.7 mm, ×2.00 k magnification, and an emission current of 9000 nA. TEM specimens were prepared by placing one drop (10 µL) of the CMP and CNT-CMP ethanol-dispersed solution onto a carbon-coated copper grid and drying it in an oven for 6 h at 60 • C. All the sample solutions were treated in an ultrasonic bath (15 min) before the deposition to reduce aggregation. TEM was performed using JEM 3010, JEOL Ltd., Japan, at 300 kV, with a total magnification of ×22.00 k and indicated magnification of ×29.00 k. UV-Vis absorption spectra were recorded on a (Varian Cary 100) spectrophotometer using ethanol as the solvent. CV, DPV, and EIS were performed using a WizMac WizEIS-1200 Premium voltammeter at room temperature in a standard three-electrode cell, where the working electrode was glassy carbon (GC) (area = 0.07 cm 2 ), the counter electrode was a Pt wire, and the Ag/AgCl/KCl (sat) electrode was used as the reference electrode.
The glassy calomel electrode was thoroughly washed with acetone, ethanol, and double distilled water, and polished by using alumina before drop casting. For casting, 0.5 mg I 2 -CMP-CNT-4 was dispersed in 0.5 mL ethanol followed by sonication for 20 min. A drop (20 µL) of well-dispersed composite material in the liquid-dispersed phase was added to the center of the glassy calomel electrode and the casted electrode was allowed to dry at room temperature. Likewise, CV comparisons for modified GCE, scan rate, the Nyquist plot, CV and DPV plot for various concentrations of DA, stability, reproducibility, and interference in PBS and FBS were conducted at 7.4 pH, respectively. For the EIS measurement of bare and modified GCE, we applied the frequency range from 0.1 to 10 5 Hz in PBS (7.4 pH). Since the pH of human blood is around 7.35-7.45, 7.4 was selected for various electrochemical measurements. Additionally, we studied the pH response in 7.62, 7.27, and 6.27 by adding dilute hydrochloric acid to the analyte solution.

Preparation of CMP-4
1,4-diethynylbenzene (50 mg, 0.396 mmol) and 1,3,5-tribromobenzene (49.8 mg, 0.158 mmol) were dissolved in a mixture of toluene (5 mL) and Et 3 N (2.5 mL) in a 50 mL glass vial. Tetrakis(triphenylphosphine)palladium (11 mg) and copper iodide (3.5 mg) were added to the brown-colored solution and purged with nitrogen gas to prevent the homocoupling of alkyne monomers. The reaction mixture was heated to 80 • C for 72 h. Subsequently, the mixture was cooled to room temperature step-by-step. The precipitated polymer was filtered through a 90 mm filter paper and washed four times with chloroform, water, methanol, and acetone. CMP-4 polymer ( Figure S2a) was purified by Soxhlet extraction from methanol for 48 h. The product dried in an oven for 6 h at 60 • C.

Preparation of CMP-CNT-4
We followed the same procedure in Section 2.1 for the synthesis of CMP-CNT-4. An extra 10 mg of CNTs was added to the brown-colored solution containing 1,4-diethynylbenzene and 1,3,5-tribromobenzene. Tetrakis(triphenylphosphine)palladium (11 mg) and copper iodide (3.5 mg) were added to the solution, which was purged with nitrogen gas. The reaction mixture was heated to 80 • C for 72 h. The precipitated polymer network was filtered and washed four times with chloroform, water, methanol, and acetone. The Soxhlet extraction ( Figure S2b) using methanol was used for further purification.

Synthesis of I 2 -CMP-CNT-4
We adopted a gravimetric method for the adsorption of iodine onto CMP-CNT-4. A vial (1.5 mL) containing 20 mg of dried CMP-CNT-4 powder was placed into a 50 mL vial, which was charged with 500 mg of iodine. Then, it was capped, heated to 35 • C, and kept in dark for 24 h, yielding black-colored iodine adsorbed I 2 -CMP-CNT-4.

Physical and Chemical Characterization of the CMP-4 and CMP-CNT-4
The optical properties of the as-synthesized COF (CMP-4) were determined using photoluminescence (PL) emission spectra. The alkyne-linked polymer exhibited a bright yellowish-green fluorescence under UV illumination ( Figure S2e, ESI †). Figure 1a shows photoexcitation at various wavelengths ranging from 290 to 410 nm. Poly(arylene-ethynylene) exhibited almost excitation-independent emission properties. The emission maximum (λmax) was 510 nm (Figure 1b) under excitation at 390 nm, owing to the π-π* transition of the conjugated π-electrons perpendicular to the molecular plane. Fluorescence is generally observed in the lowest energy transition, which is π* → π for the delocalized electrons in poly(arylene-ethylene). Figure 1c shows the UV-Vis absorption spectrum of the solid poly(arylene-ethynylene) sample dispersed in ethanol, which has a peak at 360 nm.
The carbon atoms in poly(arylene-ethynylene) are in three different chemical environments ( Figure 1d). Two highly de-shielded carbons in the aromatic ring and one triply bound, shielded alkynyl carbon outside the aromatic ring gave three distinct peaks in 13C-NMR spectra. The triply bonded carbon exhibited shifts of 89.37 and 90.36 ppm for CMP-4 and CMP-CNT-4, respectively, while the acetylene-bonded carbon within the aromatic ring showed shifts of 122.89 and 122.85 ppm. The un-bonded carbon had shifts of 130.24 and 130.84 ppm. Figure 1e shows the chemical structure of poly(arylene-ethynylene), annotated with 13C NMR shifts in ppm.
In conclusion, the synthesis of CMP-4 and CMP-CNT-4 was confirmed through physical and chemical analyses.

Morphological Characterization of the CMP-CNT-4
SEM was used to assess the surface structure and shape of as-synthesized CMP-4 and CMP-CNT-4 (Figures 2a,b and S3 (ESI †)). Analysis of the brown-colored CMP-4 revealed that the material was composed of solid spheres (with sub-micrometer dimensions), as shown in Figure 2a. The SEM image of the CMP-CNT-4 Figures 2b and S4b) nanocomposite exhibits tubular structures along with spheres, indicating the successful wrapping of CMP-4 around the CNT [27]. TEM was employed to evaluate the external morphology and imperfections of CMP-4 and CMP-CNT-4, as shown in Figure 2c,d. The TEM images were in accordance with the SEM analysis and proved that the spherical CMP-4 particles had an average size of 1 µm ( Figure S4a, ESI †). These spheres were also found to be wrapped over the CNT, yielding tubular CMP-CNT-4 structures (Figure 2d) [27]. Physical and morphological analyses confirmed the presence of CNT nanowires in the CMP-4 framework, confirming that CMP-CNT-4 was a nanocomposite.

Morphological Characterization of the CMP-CNT-4
SEM was used to assess the surface structure and shape of as-synthesized CMP-4 and CMP-CNT-4 (Figures 2a,b and S3 (ESI †)). Analysis of the brown-colored CMP-4 revealed that the material was composed of solid spheres (with sub-micrometer dimensions), as shown in Figure 2a.  and imperfections of CMP-4 and CMP-CNT-4, as shown in Figure 2c,d. The TEM images were in accordance with the SEM analysis and proved that the spherical CMP-4 particles had an average size of 1 μm ( Figure S4a, ESI †). These spheres were also found to be wrapped over the CNT, yielding tubular CMP-CNT-4 structures (Figure 2d) [27]. Physical and morphological analyses confirmed the presence of CNT nanowires in the CMP-4 framework, confirming that CMP-CNT-4 was a nanocomposite.  CNT. The XRD data confirmed that the peak detected from the composite is from the CNT-induced crystallization of CMP-4.
Raman spectroscopy was performed to further analyze the intrinsic structure of CMP-CNT-4. As shown in Figure 2f, the peak at 1350 cm −1 corresponds to the D-band, which suggests the presence of disordered carbon frameworks, while the peak at 1590 cm −1 represents the G-band, indicating the presence of sp 2 hybridized carbon in the framework. As the crystalline nature provides a smooth Raman plot for CNT ( Figure S6), the noise in the CMP-CNT-4 plot is due to the weak crystalline nature of CMP-4 (Figure 2f). Similarly, the presence of sp 3 and sp 2 carbon in the CNT gives the D and G bands in the Raman spectra. The absence of the sp 3 carbon in CMP-4 gives only the G band in the Raman spectra ( Figure S6). Overall, the intense G band compared to the D band in the composite is from the resultant peak of CNT and CMP-4 ( Figure S6).
The XPS survey spectrum (Figures 2g and S23) revealed the presence of C(1s) and I (3p, 3d, and 4d) core-shell electronic energy levels in the I 2 -CMP-CNT-4. C(1s) ( Figure S23) in CMP-CNT-4 were in three different chemical environments (1 sp and 2 sp 2 ) exhibiting a peak at 283.9, 285.4, and 287.1 eV, respectively. To be clear, carbon from the outer layer in CMP-CNT-4 showed an XPS peak for this composite. Moreover, the C(1s) peak was unresponsive after doping, confirming the physical interaction between the carbon in CMP-4 and adsorbed I 2 . In general, alkynyl bonding provided chemical stability to the CMP-CNT-4 network.
The permanent porosity of the CMP-CNT-4 network was examined by gas sorption measurements using nitrogen at 77 K after activation at 100 • C for 8 h (Figure S7a-c). The Brunauer-Emmett-Teller (BET) surface area of CMP-CNT-4 was calculated as 998.712 m 2 /g. In isotherm studies, the improved nitrogen uptake above a relative pressure of 0.2 and the increase in uptake above P/P 0 of 0.8 is due to the combination of the tubular and microporous nature of the CMP-CNT-4 network.
In summary, we synthesized I 2 -CMP-CNT-4 with a microporous size and rigid monomer, owing to its alkynyl bonding. The scan rate, which shows the pace of fluctuation of the electric potential with respect to time, is a decisive parameter in CV experiments. A study of the redox behavior of 4 µM DA in 0.1 M PBS (7.4 pH) by sweeping the voltage from 50 to 500 mV/s was performed for the I 2 -CMP-CNT-4-modified GCE. The results demonstrated that a high scan rate increased both the oxidation and reduction peak currents (Figure 3b) and caused a slight shift in the redox peak potential, owing to the smaller diffusion layer [43,44]. The kinetic behavior of the nanocomposite was calculated using the mathematical relationship between the voltammetry current response of the composite material and the scan rate. A calibration curve (Figure 3c) was plotted, and the current response exhibited a linear relationship (R 2 = 0.989) for scan rates in the range of 100-500 mV. Figure 3d shows the current vs. (scan rate) 1/2 for the diffusion mechanism. The linear plot in Figure 3c,d confirms that this process has diffusion-and adsorption-controlled mechanisms. The scan rate, which shows the pace of fluctuation of the electric potential with respect to time, is a decisive parameter in CV experiments. A study of the redox behavior of 4 μM DA in 0.1 M PBS (7.4 pH) by sweeping the voltage from 50 to 500mV/s was performed for the I2-CMP-CNT-4-modified GCE. The results demonstrated that a high scan rate increased both the oxidation and reduction peak currents (Figure 3b) and caused a slight shift in the redox peak potential, owing to the smaller diffusion layer [43,44]. The kinetic behavior of the nanocomposite was calculated using the mathematical relationship between the voltammetry current response of the composite material and the scan rate. A calibration curve (Figure 3c) was plotted, and the current response exhibited a linear relationship (R 2 = 0.989) for scan rates in the range of 100-500 mV. Figure 3d shows the current vs. (scan rate) 1/2 for the diffusion mechanism. The linear plot in Figure 3c,d confirms that this process has diffusion-and adsorption-controlled mechanisms. Since DA adopts a diffusion and adsorption-controlled mechanism towards the I 2 -CMP-CNT-4-modified GCE. This mixed kinetic mechanism is proved through 'Ip' vs. 'scan rate' and 'Ip' vs. (scan rate) 1/2 linear plot. In this context, the log(A) vs. log(V) plot further confirms the exact sensing mechanism through its slope ( Figure S10). It is well known that a slope near 1 is for adsorption controlled, and near 0.5 is for a diffusion-controlled process [35]. Figure S10 shows the relationship between log A and log V (scan rate), which follows the linear equation y = 0.6825x + 0.6325 (log(A) = 0.6825log(V) + 0.6325). Based on the log(A) vs. log(V) plot, where the slope is 0.68, it is evident that diffusion dominates over adsorption whereas, to some extent, it still shows simultaneous adsorption-and diffusion-controlled kinetics.

Electrochemical Behavior of a Modified GCE
The Nyquist plots ( Figure S11, ESI †) are the resultant Faradaic impedance spectrum, which provides information on parameters such as double-layer capacitance, Warburg diffusional impedance, and ohmic resistance [42]. It was observed that the I 2 -CMP-CNT-4, CMP-CNT-4, and CMP-4-modified GCE showed lower Ret values than the bare GCE. Interestingly, after modification of the GCE surface with CMP-4, CMP-CNT-4, and I 2 -CMP-CNT-4, the diameter of the semicircle portion of the Nyquist plot gradually decreased, which implies a gradual increase in conductivity and faster electron transfer. The tubular network of CNT and the enveloped CMP-4 enhanced the unidirectional charge mobility. Iodine serves as the charge carrier, accepting and donating electrons throughout the CMP-CNT composite.
pH is a vital parameter that significantly affects the electrochemical performance of the modified GCE. To monitor the influence of protons in an electrochemical redox reaction, the peak response towards various pH values 6.27 to 7.67 was performed in 0.1 M PBS and 4 µM DA. Figure 3d shows that the Ip of DA increased for pH values up to 5. This is due to the π-π interactions between CMP-4 and DA, as well as the adsorption of protonated DA to the CMP-CNT-4 surfaces through the lone pair of I 2 . Conversely, because the electrochemical oxidation of DA includes deprotonation, the reaction is weaker in extremely acidic environments, which leads to a drop in the peak currents [45,46].

Electrochemical Detection of DA and Sensing Mechanism
The I 2 -CMP-CNT-4-modified GCE exhibited a strong reversible peak towards DA, and the current increased gradually from 17 to 160 µA with the addition of 0.8−20 µM DA in the CV measurements (Figure 4a). To formulate the mathematical relationship between the voltammetric current response of the composite material and DA concentration, a calibration curve (Figure 4b) was plotted. The redox response showed a linear relationship with DA concentration in the range of 0.8-10 µM. CV studies clearly showed that the peak current response is highly sensitive and has good linearity with DA concentration in the range of 0.8-10 µM (R 2 = 0.9939); the limit of detection (LOD) was determined to be 1 µM. LOD was calculated based on the standard deviation of the result (Sy) and the slope of the calibration curve (S). LOD according to the formula is; Therefore, the remarkable current response of the nanocomposite compared to that of the bare GCE can be explained by its larger surface area, more favorable electron transfer, increased ability to adsorb biomolecules, and favorable environment for dopamine oxidation [43].
A more sensitive technique called DPV was applied to monitor DA oxidation, which resulted in an anodic wave at a voltage near −0.05 V. The best potential step value was derived using a pulse width of 50 ms, pulse amplitude of 20 mV, step period of 0.1 s, and step height of 100 mV in the potential range from −0.5 to +0.5 V. Quantitative measurements were performed for DA in the concentration range from 0.75 to 20 µM (Figure 4c), which shows a gradual increase in the current from 9.64 to 60 µA. As shown in Figure 4c, the peak position changed throughout the experiment, indicating that the surface was poisoned during each experimental cycle. This is due to the passivation of the electrode surface by the synthesis of melanin from DA and dopamine chrome. Melanin forms an impermeable layer that inhibits direct contact between the analyte and the electrode surface. To formulate the mathematical relationship between the voltammetric current response of the composite material and the DA concentration, a calibration curve (Figure 4d) was plotted, and the current response showed a linear relationship with the DA concentration in the range of 1-10 µM. DPV studies clearly showed that the peak current response had good linearity with DA concentrations in the range of 1-10 µM (R 2 = 0.9822); the limit of detection was determined to be 1.7 µM. Calculations based on these results suggest that the electrode reactions proceed through a two-electron transfer with the release of two protons [45].
In cyclic voltammetry measurements, the redox reaction was observed to be diffusioncontrolled; however, the DPV data indicated that DA oxidation was preceded by the adsorption of molecules onto the electrode surface [46][47][48][49][50]. Table 1 presents a comparison of the I 2 -CMP-CNT-4-modified GCE with the other modified GCEs, indicating the superiority of our material.
surface by the synthesis of melanin from DA and dopamine chrome. Melanin forms an impermeable layer that inhibits direct contact between the analyte and the electrode surface. To formulate the mathematical relationship between the voltammetric current response of the composite material and the DA concentration, a calibration curve ( Figure  4d) was plotted, and the current response showed a linear relationship with the DA concentration in the range of 1-10 μM. DPV studies clearly showed that the peak current response had good linearity with DA concentrations in the range of 1-10 μM (R 2 = 0.9822); the limit of detection was determined to be 1.7 μM. Calculations based on these results suggest that the electrode reactions proceed through a two-electron transfer with the release of two protons [45]. In cyclic voltammetry measurements, the redox reaction was observed to be diffusion-controlled; however, the DPV data indicated that DA oxidation was preceded by the adsorption of molecules onto the electrode surface [46][47][48][49][50]. Table 1 presents a comparison of the I2-CMP-CNT-4-modified GCE with the other modified GCEs, indicating the superiority of our material.   The DPV response in FBS was recorded for the real sample response of the I 2 -CMP-CNT-4-modified GCE towards DA ( Figure S12). For this study, 20 mL of FBS was directly added to 0.1M PBS (7.4 pH), and this sample was further spiked with a known concentration of DA (8-18 µM). There was an increase in the peak current response of the FBS-PBS solution according to the DA concentration, as shown in Figure S12. Moreover, a calibration curve for 'Current Vs. Concentration' (Figure S12) was plotted, where the current response showed a linear relationship with DA concentration in the range of 8-18 µM. Thus, the DPV studies clearly show that the peak current response has good linearity with DA concentrations in the range of 8-18 µM (R 2 = 0.9924).

Interference, Stability, and Reproducibility Study
Analogs and interferents curtail the detection of DA by voltammetry [59]. The DPV plot ( Figure S13) proves the insensitive nature of the I 2 -CMP-CNT-4-modified GCE towards 1 µM AA in PBS (pH 7.4). Simultaneous sensing of DA and AA was investigated through CV and DPV in the concentration range of 1-20 µM in a 0.1 M phosphate-buffered electrolyte solution. Figure 5a,b show the CV and DPV signals for DA in the presence of interfering ascorbic acid (AA). As shown in Figure 5a, the CV investigation reveals the insensitive nature of the I 2 -CMP-CNT-4-modified GCE towards AA. In the DPV measurement (Figure 5b), the I 2 -CMP-CNT-4 modified GCE exhibits two distinct peak currents (−0.3 & 0.00 V) due to AA and DA oxidation, respectively. Similarly, the interference of the modified GCE towards other anions such as sulfate, nitrate, acetate, and urea (Ur) was evaluated using CV and DPV in the presence of 1 µM DA. Figure S14a-e again confirms the insensitive nature of the I 2 -CMP-CNT-4-modified GCE. Additionally, Figure S15 displays the DPV plots of DA (1 µM), L-cysteine (L-Cyst, 1 µM), and glutamic acid (GA, 1 µM). From the DPV plot, we can observe that the oxidation peak current position of DA is distinguishable by the addition of amino acids to the PBS. However, cationic interferents ( Figure S16), such as Ca 2+ , K + , and Na + (individual concentration of 1 µM), enhanced the peak current value of the modified electrode in the DPV analysis for DA. The response to various interferents such as analog (AA), amino acid (Cyst, Argrn), cationic, and anionic (Mg 2+ , Na + , nitrate, chloride) salts were evaluated in FBS containing 6 μM DA ( Figure S17). The DPV investigation confirmed the insensitive nature of the I2-CMP-CNT-4-modified GCE towards AA, L-cystine (Cyst), arginine (Argrn), Mg 2+ , Na + , nitrate, and chloride, which is in accordance with previous results. Likewise, stability and reproducibility play a decisive role in the detection of DA in practical applications. The  The response to various interferents such as analog (AA), amino acid (Cyst, Argrn), cationic, and anionic (Mg 2+ , Na + , nitrate, chloride) salts were evaluated in FBS containing 6 µM DA ( Figure S17). The DPV investigation confirmed the insensitive nature of the I 2 -CMP-CNT-4-modified GCE towards AA, L-cystine (Cyst), arginine (Argrn), Mg 2+ , Na + , nitrate, and chloride, which is in accordance with previous results. Likewise, stability and reproducibility play a decisive role in the detection of DA in practical applications. The stability of the prepared probe was analyzed by CV by repeating the cycle at a fixed concentration of DA (4 µM) at a scan rate of 100 mV/s. Upon deducing the data, it was found that the obtained CV result had a detained current response ( Figure S18). From the data, we calculated the mean, standard deviation (SD), and relative standard deviation (RSD) as 91 ± 2 with RSD of 2.8%, respectively (n = 8 days). Similarly, the shelf life and reproducibility of the modified GCE were tested by storing the electrode at room temperature and measuring the DPV response on alternate days. For a clear study, we separately cast the electrode for 5 and 6 µM DA concentrations. From the data, the peak current is stable, in accordance with the previous results. Additionally, we calculated the mean, standard deviation (SD), and relative standard deviation (RSD) as 44 ± 2%, and 50 ± 2% with RSD of 2.69% and 2.22% for 5 and 6 µM DA, respectively (n = 8 days) (Figures S19 and S20). In brief, the nanocomposite-modified GCE exhibited excellent selectivity and sensitivity for the determination of DA, along with high reproducibility and stability. In addition, the aromatic framework of CMP induces π-π stacking interactions towards the phenyl moiety of DA and boosts the selective sensing of DA from interferents [48][49][50].

Conclusions
In this study, the CNT-embedded, weak-crystalline, two-dimensional conjugated microporous poly(arylene-ethynylene)-4 was synthesized using a one-pot solvothermal synthesis. The electrical conductivity of the COF was enhanced by doping I 2 onto the CMP-CNT-4 surface. This nanocomposite demonstrated a large increase in the anodic peak current, signifying that the as-synthesized I 2 -CMP-CNT-4 could be employed as an electrochemical sensor for the fast detection of DA. The composite provides enhanced support for the adsorption of DA and increases the mobility of electrons between the GCE and analyte, which creates a remarkable increase in the electron transfer rate compared to GCE. Moreover, this is a simple and low-cost method for the one-pot synthesis of the CMP-CNT-4-based probe for DA sensing. In addition, the prepared probe has acceptable selectivity, outstanding sensitivity, stability, reproducibility, and detection limits of 1 and 1.7 µM based on cyclic voltammetry (CV) and differential pulse voltammetry (DPV), respectively. Moreover, the current study is based on the perspective of chemistry and focuses on two areas: (1) Boosting the electrical conductivity of COF through increasing the crystallinity and incorporating charge carriers. (2) The charge transport mechanism in I 2 -CMP-CNT-4. In addition, this article provides an idea regarding the alteration of an amorphous covalent network into a crystalline structure. This crystalline modification in the network enhanced the unidirectional charge mobility.